Abstract
Enhanced microwave absorption, larger than that in the normal state, is observed in fine grains of typeII superconductors (MgB_{2} and K_{3}C_{60}) for magnetic fields as small as a few % of the upper critical field. The effect is predicted by the theory of vortex motion in typeII superconductors, however its direct observation has been elusive due to skindepth limitations; conventional microwave absorption studies employ larger samples where the microwave magnetic field exclusion significantly lowers the absorption. We show that the enhancement is observable in grains smaller than the penetration depth. A quantitative analysis on K_{3}C_{60} in the framework of the Coffey–Clem (CC) theory explains well the temperature dependence of the microwave absorption and also allows to determine the vortex pinning force constant.
Introduction
Electrodynamics of superconductors remains an intensively studied field^{1} due to the wealth of attainable fundamental information, including the nature of pairing mechanism and the coupling strength, and also due to the technological importance of these materials. In addition, recent studies focus on novel topological phases including superconductors^{2}. As an example, observation of the conductivity coherence peak in conventional superconductors^{3} (Nb and Pb) and its absence in highT_{c} materials^{4} pointed to a BCS mechanism in the former and it was an early indication of nonBCS superconductivity in the latter compounds. Concerning applications, the DC electrodynamic properties in the mixed state of typeII superconductors determine the utility (e.g. loss, permanent field homogeneity, and stability) in superconducting solenoid coils that are widely used in superconducting particle acceleration, solid state spectroscopy, or medical imaging. The AC electrodynamic properties are relevant for applications including e.g. power handling, sound and electromagnetic field detection^{5,6,7}, superconducting microwave resonators^{8}, and in microwave absorbers^{9}.
The frequency dependent conductivity of superconductors, \(\tilde{\sigma }={\sigma }_{1}+i{\sigma }_{2}\), is well known for both BCS (i.e. weakcoupled swave pairing) and nonBCS superconductors (including strongly coupled swave and non swave superconductors) in the absence of magnetic field, B = 0. At zero temperature, T = 0, the real part, σ_{1}(ω), is a delta function at ω = 0 followed by σ_{1}(ω) = 0 until the gap edge at ω_{g} = 2Δ/ℏ (ref.^{10}) (usually at 0.1–10 THz). According to the Ferrell–Glover–Tinkham (FGT) sum rule^{11,12}, the spectral weight of the delta function comes from states which are gapped below ω_{g} (the sum rule is discussed in depth in the Supplementary Material). The technologically important radio frequency range spans 9 orders of magnitude in superconductors (from 10 kHz up to 1 THz) with similar characteristic properties, thus measurements in the microwave range (1–100 GHz) are representative.
Conductivity in finite magnetic fields for the mixed state in typeII superconductors was first described by the Bardeen–Stephen (BS) model^{13} for the viscous motion of vortices. This was later improved by the Coffey–Clem theory (CC) in a series of seminal papers^{14,15,16,17,18,19}, which also includes the effect of pinning force on the vortex motion. The most important prediction of the BS model is a finite σ_{1} conductivity at ω = 0. However, it is less wellknown that the FGT sum rule implies a nonzero σ_{1} that is larger than in the normal state for ω < ω_{g}. Observation of this effect has been elusive as most contributions study the surface impedance on polycrystalline^{3}, compacted powder pellet, or thin film samples^{20,21}. Surface impedance studies have the advantage that sample geometry is well defined, however the effects of σ_{1} and σ_{2} are inevitably intermixed in this type of measurements. Given that σ_{2} is orders of magnitude larger than σ_{1} in the superconducting state (due to the small value of the penetration depth, λ, with respect to sample thickness), the surface impedance measurement is less sensitive to changes in σ_{1} (refs^{22,23,24,25,26}).
The effects of σ_{1} and σ_{2} are decoupled for fine grains; for a sample placed in a microwave cavity, the loss is due to σ_{1}, whereas the resonance shift is due to σ_{2} (refs^{27,28,29}). Therefore such samples provide a unique opportunity to test the predictions of the CC theory on σ_{1,2}(T, B). The enigmatic and yet unexplained increase of the electron spin resonance signal in superconductors right below T_{c} (refs^{30,31}) also highlights the need to study further the electromagnetic absorption in superconductors.
This motivated us to revisit the microwave conductivity (at about 10 GHz) in the MgB_{2} and K_{3}C_{60} superconductors as a function of T and B. We observe an excess microwave loss (or microwave absorption) in small magnetic fields (as low as a few % of the upper critical field, B_{c2}) for a sample consisting of wellseparated fine grains (typical size is a few micrometers). The excess microwave absorption is not observable in a single crystal sample. A quantitative analysis is provided for K_{3}C_{60}, which is a onegap, cubic superconductor with well known magnetotransport properties^{32}, whereas MgB_{2} is a multiband superconductor with strongly anisotropic B_{c2} (refs^{33,34}), thus application of the CC model is less straightforward.
Methods and Experimental
We studied fine powder MgB_{2} samples identical to batches in refs^{35} and^{30}. Single crystal and powder K_{3}C_{60} samples were prepared by the conventional K intercalation method; the crystal sample was from the same batch as in ref.^{36}. The starting fullerene powder material contains grains with a size of a few micrometers that is retained in the K doped material according to literature studies^{37,38,39}. The powder samples were further ground together with nonconducting SnO_{2} powder to prevent conducting links between the grains. Samples were sealed in quartz ampules under low pressure helium. Microwave properties were measured with the cavity perturbation method^{27,28} as a function of temperature, T, and in various static magnetic fields, B, inside a superconducting solenoid, with zerofield cooling. Zero field measurements (besides the Earth’s magnetic field) were made in another cryostat without a magnet field solenoid to avoid trapped flux (which may amount to 10–20 mT). The unloaded copper cavity has a quality factor, Q_{0} ~ 10,000 and a resonance frequency, f_{0} ~ 11.2 GHz, whose temperature dependence is taken into account. The samples were placed in the node of the microwave (or rf) electric field and maximum of the microwave magnetic field inside the TE011 cavity, which is the appropriate geometry to study minute changes in the conductivity^{29}. The rf magnetic field is parallel to the DC field of the solenoid, which yields the largest vortex motion induced absorption according to the CC theory^{16}. Measurement^{40} of the quality factor, Q, and the cavity resonance frequency, f yields the loss: \({\rm{\Delta }}(\frac{1}{2Q})=\frac{1}{2Q}\frac{1}{2{Q}_{0}}\) and cavity shift: Δf/f_{0} = (f − f_{0})/f_{0}.
Results
Figure 1 shows the microwave cavity loss and cavity shift for a fine powder of MgB_{2} and for two kinds of K_{3}C_{60} samples: a single crystal and a fine powder as a function of temperature and for a few magnetic field values. The microwave loss decreases rapidly below T_{c} in zero magnetic field as expected for superconductors. The most important observation is that the microwave loss becomes significant for a magnetic field as small as 0.1 T for the fine powder samples, whereas even 1 T has little effect on the microwave absorption for the single crystal K_{3}C_{60} sample. In fact, we observe a giant, about a factor 3 times larger, microwave absorption below T_{c} than in the normal state. This striking difference between the crystal and fine grain samples is clearly demonstrated for K_{3}C_{60} where measurements on both kinds of samples are shown. For MgB_{2}, microwave measurements on compacted samples (or surface impedance measurements) supports this observation as therein no enhanced microwave absorption was observed^{41,42,43,44,45,46}. While the absorption becomes significant for the fine powder samples at B = 0.1 T, the shift changes less, which means that the overall superconducting characteristics of the sample are maintained.
We believe that the enhanced microwave absorption is an ubiquitous property of fine powders of typeII superconductors. However, we cannot quantitatively discuss this effect for MgB_{2} due to the multiband superconductivity^{47,48} and the significant B_{c2} anisotropy; B_{c2} at 0 K is ~2 T and ~16 T for \(B\parallel (c)\) and \(B\parallel (a,b)\), respectively (refs^{34,35,49}). We therefore focus on K_{3}C_{60} in the following. The enhanced microwave loss appears progressively with increasing magnetic field (additional data are shown in the Supplementary Material).
We also show the B = 0.1 T data for the powder sample (B ≈ 0.002 × B_{c2}) in Fig. 1; they show a peak in the microwave loss right below T_{c} followed by a gradual decrease. The zero magnetic field data also shows a small peak (invisible at the scale of Fig. 1) for the powder sample (shown in the Supplementary Material). This small peak is not due to magnetic field and is most probably a tiny conductivity coherence peak (the analogue of the Hebel–Slichter peak^{50}) which is known to be strongly suppressed by strongcoupling effects in alkali fullerides^{51,52}. While the presence of a coherence peak itself is an interesting physical phenomenon^{3,53}, it is not relevant for the present discussion.
The fact that the enhanced microwave absorption occurs with the application of the magnetic field hints at a flux motion related phenomenon that is discussed in the framework of the CC theory. The microwave absorption peak occurs above the irreversibility line, i.e. it is related to the physical behavior of the vortexfluid state; for K_{3}C_{60} T_{irr}(B = 0.1 T) ≈ 15 K and T_{irr}(B = 1 T) < 5 K (ref.^{54}).
The strong dependence on the sample morphology is also discussed below. Superconducting fullerides are typeII (\(\lambda \gg \xi \)) and have a short mean free path^{32} i.e. they can be described in the local electrodynamics limit as opposed to the nonlocal (or Pippard) limit, which simplifies the discussion.
Discussion
Conductivity in the superconducting state
The phenomenological CC theory^{14,15,16,17,18,19} is based on a twofluid model and considers the motion of vortices due to the exciting electromagnetic field in the presence of a viscous background (described by the viscous drag coefficient, η) and a restoring force (described by an effective pinning force constant, κ_{p}).
The viscous drag was introduced in the Bardeen–Stephen theory^{13} and is determined by the superconducting parameters^{10,55}: \(\eta (T)=\frac{{{\rm{\Phi }}}_{0}{B}_{{\rm{c}}2}(T)}{{\rho }_{{\rm{n}}}(T)}\). The value of κ_{p} is unknown and only an upper limit can be estimated from thermodynamic considerations^{55,56,57} for a “perfect pinning center”, i.e. a hollow cylinder with a diameter of about the coherence length, d ≈ ξ. The condensation energy gain per unit length from placing a vortex in this cylinder is about \({d}^{2}{B}_{{\rm{c}}}^{2}\mathrm{/2}{\mu }_{0}\), where the square of the thermodynamic critical field is \({B}_{{\rm{c}}}^{2}={B}_{{\rm{c}}1}{B}_{{\rm{c}}2}/\,\mathrm{ln}(\frac{\lambda }{\xi })\). This leads to:
For a weaker pinning center, κ_{p} can be significantly lower and in the bulk of a perfect superconductor, it would be zero.
The CC theory introduces the concept of the complex penetration depth, \(\tilde{\lambda }\):
where \({\tilde{\delta }}_{{\rm{nf}}}\) is the normal fluid skin depth, λ is the usual (real) penetration depth and \({\tilde{\delta }}_{{\rm{vc}}}\) is the complex effective skin depth^{19}. The latter quantity is zero for B = 0 and becomes finite in the mixed state when vortex motion is present. \(\tilde{<mml:mpadded xmlns:xlink="http://www.w3.org/1999/xlink" voffset="0">\lambda</mml:mpadded>}\) is related to the complex conductivity by \(\tilde{\sigma }=i/{\mu }_{0}\omega {\tilde{<mml:mpadded xmlns:xlink="http://www.w3.org/1999/xlink" voffset="0">\lambda</mml:mpadded>}}^{2}\). Note that for B = 0 (i.e. when \({\tilde{\delta }}_{{\rm{vc}}}^{2}=0\)), we obtain \({\tilde{<mml:mpadded xmlns:xlink="http://www.w3.org/1999/xlink" voffset="0">\lambda</mml:mpadded>}}^{2}(T=0)={\lambda }^{2}\) and \({\tilde{<mml:mpadded xmlns:xlink="http://www.w3.org/1999/xlink" voffset="0">\lambda</mml:mpadded>}}^{2}(T={T}_{{\rm{c}}})={\rm{i}}{\delta }_{{\rm{n}}}^{2}/2\) as expected. The CC theory yields the temperature and magnetic field dependent \(\tilde{\sigma }\) using explicit expressions for λ(T), δ_{nf}(T), B_{c2}(T). We have implemented the calculation (details are given in the Supplementary Material) and validated our calculations by comparing the results to that published in ref.^{19}.
Here, we discuss qualitatively the predictions of the CC theory and some typical cases are shown in Fig. 2. In superconductors, at B = 0 the carrier spectral weight below ω_{g} collapses into the \({\sigma }_{1}=\frac{\pi }{2{\mu }_{0}{\lambda }^{2}}\delta (\omega )\) function according to the Ferrell–Glover–Tinkham (FGT) sum rule^{11,12}. The Kramers–Kronig relation dictates that σ_{2} = 1/μ_{0}ωλ^{2}. Without vortex pinning, the Meissner state is destroyed for B > B_{c1} and the Bardeen–Stephen theory gives \(\sigma =\frac{{B}_{{\rm{c}}2}}{B}\frac{{\sigma }_{{\rm{n}}}}{1+{\rm{i}}\frac{\omega }{{\omega }_{{\rm{c}}}}}\). It is worth noting that this result is formally analogous to the AC Drude model as the underlying equation of motion (of electrons or vortices) is the same. Here, we introduced a cutoff frequency \({\omega }_{{\rm{c}}}=\frac{B}{{\mu }_{0}{\lambda }^{2}{B}_{{\rm{c2}}}{\sigma }_{{\rm{n}}}}\). Clearly, σ_{1} can be larger than σ_{n} for ω < ω_{c}.
In the presence of vortex pinning, the CC theory predicts that \(\tilde{\sigma }\) is characterized by a mixture of the unperturbed superconducting behavior and that of the Bardeen–Stephen theory with a shared spectral weight which depends on the pinning force constant. Pinning reduces the effect of the vortex flow on σ_{1}. The enhanced σ_{1}(ω) AC conductivity (as compared to the normal state) is a direct consequence of the FGT sum rule for a finite magnetic field. It allows to estimate the maximum possible value of the enhancement as σ_{1, max}(ω) ≈ σ_{n} × ω_{g}/ω, that would be realized at T = 0 in the absence of pinning. E.g. for K_{3}C_{60} and ω/2π = 10 GHz we obtain σ_{1, max}(ω) ≈ 140σ_{n}.
The CC theory allows to quantitatively analyze the conductivity in K_{3}C_{60}. The requirement of \(B\gg {B}_{{\rm{c1}}}\) is satisfied for our magnetic fields of 0.1 … 1 T as B_{c1} ~ 10 mT. The CC theory was developed for a superconductor which occupies the total half space. We show in the Supplementary Material that it can be applied for a spherical sample which approximates well finite sized grains containing at least a few hundred/thousand vortices. In addition, the static and rf magnetic fields are parallel in our experiment, which is the standard case for the applicability of the CC theory. Albeit we cannot quantitatively consider the effect of the small particle size on the magnetic properties, we believe that neither the surface barriers (also known as BeanLivingstone barriers^{58}) nor the socalled geometrical barriers^{59} affect considerably the applicability of the CC theory. The argument is that both types of barriers would affect the overall number of the vortices under the applied DC magnetic field (or the B value where vortices appear) but not the overall vortex dynamics under the application of the small AC magnetic field, which is the primary reason for the observed microwave absorption.
In Fig. 3, the calculated conductivity is plotted versus the reduced temperature for different force constants, κ_{p}, with the parameters ξ_{0} = 3 nm (which corresponds to B_{c2}(0 K) = 37.5 T), λ_{0} = 440 nm, and ρ_{n}(T_{c}) = 2.95 Ωm, the mean values of the corresponding literature parameters for K_{3}C_{60} (refs^{32,37,38,39,60,61,62}), which are detailed in Table 1. The pinning force constant is given in the figure with respect to \({\kappa }_{{\rm{p}},{\rm{\max }}}=3.84\cdot {10}^{4}\,{\rm{N}}/{{\rm{m}}}^{2}\) according to Eq. (1). The figure indicates that κ_{p} strongly affects the magnetic field dependence of \(\tilde{\sigma }\).
Analysis of the experimental data
The sample morphology greatly affects the relation between the material conductivity, \(\tilde{\sigma }\), and the microwave parameters, the loss and shift. Two limiting cases are known. 1) The sample is large and the field penetrates into a limited distance from the surface. This approximates the measurement in the large K_{3}C_{60} single crystal. 2) The sample is a small sphere with radius comparable to the penetration depth. This approximates the K_{3}C_{60} sample of well divided small grains. We discuss that the experimental observations for the crystal and fine powder K_{3}C_{60} are explained well by these two regimes.
In the first case, when the rf field penetrates in the skin depth only (known as the skin limit), the following equation holds between the microwave measurement parameters and the material quantities^{28}:
where the complex penetration depth, \(\tilde{<mml:mpadded xmlns:xlink="http://www.w3.org/1999/xlink" voffset="0">\lambda</mml:mpadded>}\), is related to the conductivity as \({\tilde{<mml:mpadded xmlns:xlink="http://www.w3.org/1999/xlink" voffset="0">\lambda</mml:mpadded>}}^{2}={\rm{i}}{({\mu }_{{\rm{0}}}\omega \tilde{\sigma })}^{1}\). The dimensionless \(\nu \ll 1\) is the socalled resonator constant^{3} and it depends on the sample surface relative to that of the cavity.
The left panels in Fig. 4. show the calculated and measured cavity loss and shift in 0 and 1 T magnetic fields for the single crystal sample. The calculation uses Eq. (3) with κ_{p} = κ_{p,max}/20. Although this low κ_{p} induces a large σ_{1}, there is no visible peak in the cavity loss in this case when excitation is limited to the surface. We discuss in detail in the Supplementary Material that the calculated cavity loss and shift are insensitive to the value of κ_{p} in this limit. Clearly, the experimental data for the K_{3}C_{60} crystal match well the calculations.
A suitable \(\nu =5.1\cdot {10}^{4}\) was chosen to match the calculation to the experiment. We find that for both the calculation and experiment, the cavity loss parameter drops rapidly below T_{c}, although σ_{1}/σ_{n} is around unity due to the vortex motion. This effect is due to the development of a significant σ_{2}/σ_{n} ~ 100, which limits the penetration of microwaves into the sample and thus reduces the loss. This means that the microwave surface impedance measurement is not capable of providing information about σ_{1} in the presence of vortex motion. We note that the experimental curves do not show such a rapid change as a function of temperature as the calculation. This may be related to the finite size and surface roughness of the single crystal sample.
Second, we discuss the opposite limit, when the microwave field penetrates into the sample (known as the penetration limit), the cavity measurables depend differently on the sample parameters. It was shown^{63} for a sphere with radius, a:
where \(\tilde{k}=\tilde{n}\frac{\omega }{c}\) is the complex wavenumber, with \(\tilde{n}=\sqrt{{\rm{i}}\tilde{\sigma }/{\varepsilon }_{0}\omega }\) being the complex index of refraction. The dimensionless γ is a sample volume dependent constant.
The right panels in Fig. 4, show the measured cavity loss and shift data for the fine powder sample together with a fit according to Eq. (5). To obtain these fits, we fixed the transport and magnetic parameters (ρ_{n}, ξ_{0}, λ_{0}) of K_{3}C_{60} to the respective mean values as given in Table 1. We assumed that the sample consists of spheres with a uniform diameter, a. The zero magnetic field data depends only on γ and a when the other parameters, δ_{n} and λ, are fixed. A fit to the B = 0 data yields \(\gamma =\mathrm{5.5(2)}\cdot {10}^{4}\), and a = 6.2(2) μm. We then proceed to fit the magnetic field dependent data with κ_{p} as the only free parameter and we obtain \({\kappa }_{{\rm{p}}}=\mathrm{1.0(1)}\cdot {10}^{3}\) N/m^{2}, which is about κ_{p,max}/20. As shown in Fig. 4, the calculation agrees well with the experimental data. The presence of a finite microwave absorption at B = 1 T down to the lowest temperature appears to be surprising; its origin is therefore discussed qualitatively. Although the penetration depth due to superconductivity becomes smaller than the particle size, it is accompanied by a large (σ_{1}/σ_{n} ≈ 30) conductivity due to the vortex motion. It means that a substantial microwave absorption occurs on the surface of the sample. The important observation is that the loss remains proportional to σ_{1} in this case, although its effect is reduced. This is further elaborated in the last part of the Supplementary Material.
Somewhat better fits could be obtained when letting λ, ρ_{n}, and B_{c2} differ from the mean literature values. In addition, Eq. (5) is valid for spheres only, it thus fixes the ratio between the real and imaginary parts (cavity loss and shift). A different particle shape or particle size distribution would allow for a different scaling factor for the loss and shift data which could also improve the fits. Although improved fits could be attained, we believe that the simplest model explains well the experimental observation of an enhanced microwave absorption. In addition it allows to determine an effective pinning force constant, which is an important parameter to describe the electrodynamics of typeII superconductors. However, we note that κ_{p} determined herein may overestimate the bulk pinning force constant; it is known that the presence of a substantial surfacevolume ratio may give rise to additional vortex pinning^{58,59}, with a strength that is difficult to estimate.
Summary
We demonstrated that moderate magnetic fields, which are small compared to the upper critical field, induces a large microwave absorption in fine powders of type II superconductors, like MgB_{2} and K_{3}C_{60}. The effect is absent for samples containing larger grains or compacted powder pellets. The Bardeen–Stephen model of fluxflow predicts that the real part of the AC conductivity can be enhanced in the microwave range, but this effect has not been observed. We analyze the conductivity using the Coffey–Clem theory which also accounts for vortex pinning effects. It is applied to calculate the microwave properties for two kinds of samples: when the electromagnetic field penetration is limited to the surface (skin limit) or when it fully penetrates into the fine grain samples (penetration limit). We show that microwave absorption in the skin limit is little affected by the vortexmotion enhanced σ_{1} but in the penetration limit, the effect is clearly observable. A quantitative analysis for K_{3}C_{60} yields the vortex pinning force constant that can be hardly determined by other means. Our observation allowed us to explain longstanding microwave anomalies in superconductors^{30,31} and it may lead to pertinent applications in microwave communication techniques.
References
 1.
Dressel, M. Electrodynamics of Metallic Superconductors. Adv. Cond. Mat. Phys. (2013).
 2.
Villegas, K. H. A., Kovalev, V. M., Kusmartsev, F. V. & Savenko, I. G. Shedding light on topological superconductors. arXiv:1805.03177.
 3.
Klein, O., Nicol, E. J., Holczer, K. & Grüner, G. Conductivity coherence factors in the conventional superconductors Nb and Pb. Phys. Rev. B 50, 6307–6316 (1994).
 4.
Nuss, M., Mankiewich, P., Omalley, M., Westerwick, E. & Littlewood, P. Dynamic Conductivity and “Coherence Peak” in YBa_{2}Cu_{3}O_{7} Superconductors. Phys. Rev. Lett. 66, 3305–3308 (1991).
 5.
Semenov, A., Gol’tsman, G. & Korneev, A. Quantum detection by current carrying superconducting film. Physica C 351, 349–356 (2001).
 6.
Baek, B., Lita, A. E., Verma, V. & Nam, S. W. Superconducting aW_{x}Si_{1−x} nanowire singlephoton detector with saturated internal quantum efficiency from visible to 1850 nm. Applied Physics Letters 98 (2011).
 7.
Wei, J. et al. Ultrasensitive hotelectron nanobolometers for terahertz astrophysics. Nature Nanotechnology 3, 496–500 (2008).
 8.
Lancaster, M. J. Passive Microwave Device Applications of HighTemperature Superconductors. (Cambridge University Press, Cambridge, UK, 2006).
 9.
Lin, T. S., Sobotka, L. G. & Froncisz, W. Superconductivity and microwave absorption. Nature 333, 21–22 (1988).
 10.
Tinkham, M. Introduction to superconductivity (Krieger Publishing Company, 1975).
 11.
Ferrell, R. A. & Glover, R. E. Conductivity of Superconducting Films: A Sum Rule. Phys. Rev. 109, 1398–1399 (1958).
 12.
Tinkham, M. & Ferrell, R. A. Determination of the Superconducting Skin Depth from the Energy Gap and Sum Rule. Phys. Rev. Lett. 2, 331–333 (1959).
 13.
Bardeen, J. & Stephen, M. J. Theory of the Motion of Vortices in Superconductors. Phys. Rev. 140, A1197–A1207 (1965).
 14.
Coffey, M. W. & Clem, J. R. Unified Theory of Effects of Vortex Pinning and Flux Creep upon the rf Surface Impedance of TypeII Superconductors. Phys. Rev. Lett. 67, 386–389 (1991).
 15.
Coffey, M. W. & Clem, J. R. Theory of rf magnetic permeability of isotropic typeII superconductors in parallel field. Phys. Rev. B 45, 9872–9881 (1992).
 16.
Coffey, M. W. & Clem, J. R. Theory of rf magnetic permeability of typeII superconductors in slab geometry with an oblique applie static magnetic field. Phys. Rev. B 45, 10527–10535 (1992).
 17.
Coffey, M. W. & Clem, J. R. Coupled nonlinear electrodynamics of typeII superconductors in the mixed state. Phys. Rev. B 46, 567–570 (1992).
 18.
Coffey, M. W. & Clem, J. R. Theory of highfrequency linear response of isotropic typeII superconductors in the mixed state. Phys. Rev. B 46, 11757–11764 (1992).
 19.
Coffey, M. W. & Clem, J. R. Theory of microwave transmission and reflection in typeII superconductors in the mixed state. Phys. Rev. B 48, 342–350 (1993).
 20.
Jin, B. B. et al. Anomalous Coherence Peak in the Microwave Conductivity of cAxis Oriented MgB_{2} Thin Films. Phys. Rev. Lett. 91, 127006 (2003).
 21.
Janjušević, D. et al. Microwave response of thin niobium films under perpendicular static magnetic fields. Phys. Rev. B 74, 104501 (2006).
 22.
Henderson, W., Andrei, E. Y., Higgins, M. J. & Bhattacharya, S. ac Dynamics of a Pinned FluxLine Lattice. Phys. Rev. Lett. 80, 381–384 (1998).
 23.
Revenaz, S., Oates, D. E., LabbléLavigne, D., Dresselhaus, G. & Dresselhaus, M. S. Frequency dependence of the surface impedance of YBA_{2}Cu_{3}O_{7−δ} thin films in dc magnetic field: Investigation of vortex dynamics. Phys. Rev. B 50, 1178–1189 (1994).
 24.
Belk, N., Oates, D. E., Feld, D. A., Dresselhaus, G. & Dresselhaus, M. S. Frequency and temperature dependence of the microwave surface impedance of YBa_{2}Cu_{3}O_{2−δ} thin films in dc magnetic field: Investigation of vortex dynamics. Phys. Rev. B 53, 1178–1189 (1996).
 25.
Parks, B. et al. PhaseSensitive Measurments of Vortex Dynamics in the Terahertz Domain. Phys. Rev. Lett. 74, 3265–3268 (1995).
 26.
Pambianchi, M. S., Wu, D. H., Ganapathi, L. & Anlage, S. M. Dc magnetic field dependence of the surface impedance in superconducting parallel plate transmission line resonators. IEEE Trans. Appl. Supercond. 3, 2774–2777 (1993).
 27.
Buravov, L. I. & Shchegolev, I. F. Instrum. Exp. Tech. 14, 528 (1971).
 28.
Klein, O., Donovan, S., Dressel, M. & Grüner, G. Microwave cavity perturbation technique: Part I: Principles. Int. J. Infr. Mill. Wav. 14, 2423–2457 (1993).
 29.
Kitano, H. et al. Evidence for Insulating Behavior in the Electric Conduction of NH_{3}K_{3}C_{60} Systems. Phys. Rev. Lett. 88, 096401 (2002).
 30.
Simon, F. et al. Magneticfieldinduced density of states in MgB_{2}: Spin susceptibility measured by conductionelectron spin resonance. Phys. Rev. B 72, 012511 (2005).
 31.
Murányi, F., Urbanik, G., Kataev, V. & Büchner, B. Electron spin dynamics of the superconductor CaC_{6} probed by ESR. Phys. Rev. B 77, 024507 (2008).
 32.
Gunnarsson, O. Superconductivity in fullerides. Rev. Mod. Phys. 69, 575–606 (1997).
 33.
Nagamatsu, J., Nakagawa, N., Muranaka, T., Zenitani, Y. & Akimitsu, J. Superconductivity at 39 K in magnesium diboride. Nature 410, 63–64 (2001).
 34.
Buzea, C. & Yamashita, T. Review of the superconducting properties of MgB_{2}. Super. Sci. Technol. 14, R115–R146 (2001).
 35.
Simon, F. et al. Anisotropy of superconducting MgB_{2} as seen in electron spin resonance and magnetization data. Phys. Rev. Lett. 87 (2001).
 36.
Nemes, N. M. et al. Conductionelectron spin resonance in the superconductor K_{3}C_{60}. Phys. Rev. B 61, 7118–7121 (2000).
 37.
Johnson, C. E. et al. Uppercriticalfieldtemperature phase diagram of alkalimetalintercalated C60 superconductors. Phys. Rev. B 46, 5880–5882 (1992).
 38.
Holczer, K., Klein, O. & Grüner, G. Critical Magnetic Fields in the Superconducting State of K_{3}C_{60}. Phys. Rev. Lett. 67, 271–274 (1991).
 39.
Uemura, Y. J. et al. Magneticfield penetration depth in K_{3}C_{60} measured by muon spin relaxation. Nature 352, 605–607 (1991).
 40.
Nebendahl, B., Peligrad, D.N., Pozek, M., Dulcic, A. & Mehring, M. An ac method for the precise measurement of Qfactor and resonance frequency of a microwave cavity. Rev. Sci. Instrum. 72, 1876 (2001).
 41.
Zhukov, A. et al. Microwave surface resistance of MgB_{2}. Appl. Phys. Lett. 80, 2347–2349 (2002).
 42.
Dulcic, A. et al. Magnetization and microwave study of superconducting MgB_{2}. Phys. Rev. B 66 (2002).
 43.
Gallitto, A., Fricano, S., Vigni, M., Kolesnikov, N. & Kulakov, M. Magnetic field dependence of the microwave surface resistance in MgB_{2} superconductors. Int. J. Mod. Phys. B 16, 1571–1576 (2002).
 44.
Nefyodov, Y. et al. Characteristic features of the temperature dependence of the surface impedance in polycrystalline MgB_{2} samples. Eur. Phys. Lett. 58, 422–428 (2002).
 45.
Hakim, N. et al. The superconducting gap of in situ MgB_{2} thin films by microwave surface impedance measurements. Appl. Phys. Lett. 81, 3603–3605 (2002).
 46.
Jin, B. et al. Energy gap, penetration depth, and surface resistance of MgB_{2} thin films determined by microwave resonator measurements. Phys. Rev. B 66 (2002).
 47.
Liu, A., Mazin, I. & Kortus, J. Beyond Eliashberg superconductivity in MgB_{2}: Anharmonicity, twophonon scattering, and multiple gaps. Phys. Rev. Lett. 87 (2001).
 48.
Choi, H., Roundy, D., Sun, H., Cohen, M. & Louie, S. The origin of the anomalous superconducting properties of MgB_{2}. Nature 418, 758–760 (2002).
 49.
Bud’ko, S. L., Kogan, V. G. & Canfield, P. C. Determination of superconducting anisotropy from magnetization data on random powders as applied to LuNi_{2}B_{2}C, YNi_{2}B_{2}C, and MgB_{2}. Phys. Rev. B 64, 180506 (2001).
 50.
Hebel, L. C. & Slichter, C. P. Nuclear Spin Relaxation in Normal and Superconducting Aluminum. Phys. Rev. 113, 1504–1519 (1959).
 51.
MacFarlane, W. A. et al. Muonspinrelaxation studies of the alkalifulleride superconductors. Phys. Rev. B 58, 1004–1024 (1998).
 52.
Pennington, C. H. & Stenger, V. A. Nuclear magnetic resonance of C_{60} and fulleride superconductors. Rev. Mod. Phys. 68, 885 (1996).
 53.
Thiemann, M., Dressel, M. & Scheffler, M. arXiv:1803.02736.
 54.
Prassides, K. Physics and Chemistry of the Fullerenes. (SpringerVerlag, Berlin, Heidelberg, 2012).
 55.
Lévy, L.P. Magnetism and Superconductivity. (SpringerVerlag, Berlin, Heidelberg, 2000).
 56.
Anderson, P. Theory of flux creep in hard superconductors. Phys. Rev. Lett. 9, 309–311 (1962).
 57.
Wu, D.H. & Sridhar, S. Pinning forces and lower critical fields in YBa_{2}Cu_{3}O_{y} crystals: Temperature dependence and anisotropy. Phys. Rev. Lett. 65, 2074–2077 (1990).
 58.
Bean, C. P. & Livingston, J. D. Surface Barrier in TypeII Superconductors. Phys. Rev. Lett. 12, 14–16 (1964).
 59.
Zeldov, E. et al. Geometrical Barriers in HighTemperature Superconductors. Phys. Rev. Lett. 73, 1428–1431 (1994).
 60.
Dra, B. & Simon, F. ElectronSpin Dynamics in Strongly Correlated Metals. Phys. Rev. Lett. (2009).
 61.
Klein, O. & Grüner, G. Elecrical resistivity of K_{3}C_{60}. Phys. Rev. B (1992).
 62.
Tycko, R. et al. Electronic Properties of Normal Superconducting Alkali Fullerides Probed by 13C Nuclear Magnetic Resonance. Phys. Rev. Lett. 68, 1912–1915 (1992).
 63.
Landau, L. D. & Lifschitz, E. M. Electrodynamics of Continuous Media, Course of Theoretical Physics 8 (Pergamon Press, Oxford, UK, 1984).
Acknowledgements
Stimulating discussions with Károly Holczer are appreciated. Support by the National Research, Development and Innovation Office of Hungary (NKFIH) Grant Nrs. K119442, SNN118012 and 20171.2.1NKP201700001, and by the Spanish MINECO Grant Nr: MAT201784496R are acknowledged. This work (P.C.C., S.L.B., and V.G.K.) was supported by the U.S. Department of Energy, Office of Basic Energy Science, Division of Materials Sciences and Engineering. The research was performed at the Ames Laboratory which is operated for the U.S. Department of Energy by Iowa State University under Contract No. DEAC0207CH11358.
Author information
Affiliations
Contributions
G.C. implemented the CC calculations, which were verified by B.G.M. under the supervision of F.S., A.J. and F.M. contributed to the microwave impedance measurements. N.M.N. prepared and characterized the single crystal K_{3}C_{60}. G.K. and K.K. prepared and characterized the fine powder K_{3}C_{60} samples. S.L.B. and P.C.C. prepared and characterized the MgB_{2} sample. V.G.K. helped the theoretical discussion in the paper. All authors contributed to writing of the manuscript.
Corresponding author
Correspondence to F. Simon.
Ethics declarations
Competing Interests
The authors declare no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Received
Accepted
Published
DOI
Further reading

Electronic Properties of AirSensitive Nanomaterials Probed with Microwave Impedance Measurements
physica status solidi (b) (2018)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.